LMucko/crystallography-open-database huggingface dataset:
A ternary alloy with Pb Cl2 - type structure: Ti Ni Si(e)
Shoemaker, C.B.; Shoemaker, D.P.; Acta Crystallographica (1,1948-23,1967) 18 (1965) 900–905; doi:

data_2310665
_publ_section_title
;
 A ternary alloy with Pb Cl2 - type structure: Ti Ni Si(e)
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              900
_journal_page_last               905
_journal_volume                  18
_journal_year                    1965
_chemical_formula_sum            'Ni Si Ti'
_chemical_name_systematic        'Ti Ni Si'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2n'
_symmetry_space_group_name_H-M   'P n a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.1484
_cell_length_b                   7.0173
_cell_length_c                   3.6698
_cell_volume                     158.334
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Shoemaker_ACCRA9_1965_1889.cif
_cod_data_source_block           Ni1Si1Ti1
_cod_original_cell_volume        158.3341
_cod_original_sg_symbol_Hall     '-P 2ac 2n (-x,z,y)'
_cod_original_formula_sum        'Ni1 Si1 Ti1'
_cod_database_code               2310665
Synthesis and structure investigation of the Pb3 V (P O4)3 eulytite
Shpanchenko, R.V.; Panin, R.V.; Hadermann, J.; Bougerol, C.; Antipov, E.V.; Takayama-Muromachi, E.; Journal of Solid State Chemistry 178 (2005) 3715–3721; doi:

data_1528884
_publ_section_title
;
 Synthesis and structure investigation of the Pb3 V (P O4)3 eulytite
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              3715
_journal_page_last               3721
_journal_volume                  178
_journal_year                    2005
_chemical_formula_sum            'O10.86 P3 Pb3 V'
_chemical_name_systematic        'Pb3 V (P O4)3'
_space_group_IT_number           220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.127
_cell_length_b                   10.127
_cell_length_c                   10.127
_cell_volume                     1038.586
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Shpanchenko_JSSCBI_2005_712.cif
_cod_data_source_block           O10.86P3Pb3V1
_cod_original_formula_sum        'O10.86 P3 Pb3 V1'
_cod_database_code               1528884
General route to three-dimensional framework uranyl transition metal phosphates with atypical structural motifs: the case examples of Cs2 {(U O2)4 [Co (H2 O)2]2 (H P O4) (P O4)4} and Cs(3+x) [(U O2)3 Cu H(4-x) (P O4)5].H2 O
Shvareva, T.Y.; Albrecht-Schmitt, T.E.; Inorganic Chemistry 45 (2006) 1900–1902; doi:

data_4343905
_publ_section_title
;
 General route to three-dimensional framework uranyl transition metal
 phosphates with atypical structural motifs: the case examples of Cs2 {(U
 O2)4 [Co (H2 O)2]2 (H P O4) (P O4)4} and Cs(3+x) [(U O2)3 Cu H(4-x) (P
 O4)5].H2 O
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1900
_journal_page_last               1902
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cs3.14 Cu H5.86 O27 P5 U3'
_chemical_name_systematic        'Cs3.14 ((U O2)3 Cu H3.86 (P O4)5) (H2 O)'
_space_group_IT_number           57
_symmetry_space_group_name_Hall  '-P 2c 2b'
_symmetry_space_group_name_H-M   'P b c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.5867
_cell_length_b                   19.9574
_cell_length_c                   17.9726
_cell_volume                     2721.246
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Shvareva_INOCAJ_2006_723.cif
_cod_data_source_block           H5.86Cs3.14Cu1O27P5U3
_cod_original_formula_sum        'H5.86 Cs3.14 Cu1 O27 P5 U3'
_cod_database_code               4343905
_cod_duplicate_entry 4331940
Neutron diffraction studies of hafnium-hydrogen and titanium-hydrogen systems
Sidhu, S.S.; Heaton, L.R.; Zauberis, D.D.; Acta Crystallographica (1,1948-23,1967) 9 (1956) 607–614; doi:

data_2310666
_publ_section_title
;
 Neutron diffraction studies of hafnium-hydrogen and titanium-hydrogen
 systems
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              607
_journal_page_last               614
_journal_volume                  9
_journal_year                    1956
_chemical_formula_sum            'D1.628 Hf'
_chemical_name_systematic        'Hf D1.628'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.681
_cell_length_b                   4.681
_cell_length_c                   4.681
_cell_volume                     102.569
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Sidhu_ACCRA9_1956_201.cif
_cod_data_source_block           D1.628Hf1
_cod_original_formula_sum        'D1.628 Hf1'
_cod_database_code               2310666
Heterobimetallische 3d-4f-Komplexe mit bis(1,2-dithiooxalato)nickelat(II) als planarem Brueckenbaustein
Siebold, M.; Kelling, A.; Schilde, U.; Strauch, P.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 60 (2005) 1149–1157; doi:

data_7221510
_publ_section_title
;
 Heterobimetallische 3d-4f-Komplexe mit bis(1,2-dithiooxalato)nickelat(II)
 als planarem Brueckenbaustein
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1149
_journal_page_last               1157
_journal_volume                  60
_journal_year                    2005
_chemical_formula_sum            'C12 H28 Nd2 Ni3 O34 S12'
_chemical_name_systematic        '(Nd (H2 O)5)2 (Ni (S2 C2 O2)2)3 (H2 O)12'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.907
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.3987
_cell_length_b                   11.4878
_cell_length_c                   20.823
_cell_volume                     2457.481
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Siebold_ZNBSEN_2005_975.cif
_cod_data_source_block           C12H28Nd2Ni3O34S12
_cod_database_code               7221510
Heterobimetallische 3d-4f-Komplexe mit bis(1,2-dithiooxalato)nickelat(II) als planarem Brueckenbaustein
Siebold, M.; Kelling, A.; Schilde, U.; Strauch, P.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 60 (2005) 1149–1157; doi:

data_7221511
_publ_section_title
;
 Heterobimetallische 3d-4f-Komplexe mit bis(1,2-dithiooxalato)nickelat(II)
 als planarem Brueckenbaustein
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1149
_journal_page_last               1157
_journal_volume                  60
_journal_year                    2005
_chemical_formula_sum            'C12 H36 Er2 Ni3 O30 S12'
_chemical_name_systematic        '(Er (H2 O)5)2 (Ni (S2 C2 O2)2)3 (H2 O)8'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                107.899
_cell_angle_beta                 91.436
_cell_angle_gamma                112.918
_cell_formula_units_Z            1
_cell_length_a                   10.5091
_cell_length_b                   11.0604
_cell_length_c                   11.2823
_cell_volume                     1133.636
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Siebold_ZNBSEN_2005_976.cif
_cod_data_source_block           C12H36Er2Ni3O30S12
_cod_database_code               7221511
The crystal structure of K Br F4
Siegel, S.; Acta Crystallographica (1,1948-23,1967) 9 (1956) 493–495; doi:

data_2310667
_publ_section_title
;
 The crystal structure of K Br F4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              493
_journal_page_last               495
_journal_volume                  9
_journal_year                    1956
_chemical_formula_sum            'Br F4 K'
_chemical_name_systematic        'K (Br F4)'
_space_group_IT_number           140
_symmetry_space_group_name_Hall  '-I 4 2c'
_symmetry_space_group_name_H-M   'I 4/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.174
_cell_length_b                   6.174
_cell_length_c                   11.103
_cell_volume                     423.227
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Siegel_ACCRA9_1956_194.cif
_cod_data_source_block           Br1F4K1
_cod_original_cell_volume        423.2272
_cod_original_formula_sum        'Br1 F4 K1'
_cod_database_code               2310667
The structures of Cs2 Th Cl6 and Cs2 U Cl6
Siegel, S.; Acta Crystallographica (1,1948-23,1967) 9 (1956) 827–827; doi:

data_2310668
_publ_section_title
;
 The structures of Cs2 Th Cl6 and Cs2 U Cl6
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              827
_journal_page_last               827
_journal_volume                  9
_journal_year                    1956
_chemical_formula_sum            'Cl6 Cs2 Th'
_chemical_name_systematic        'Cs2 Th Cl6'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   7.614
_cell_length_b                   7.614
_cell_length_c                   6.038
_cell_volume                     303.144
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Siegel_ACCRA9_1956_209.cif
_cod_data_source_block           Cl6Cs2Th1
_cod_original_cell_volume        303.1443
_cod_original_formula_sum        'Cl6 Cs2 Th1'
_cod_database_code               2310668
The structures of Cs2 Th Cl6 and Cs2 U Cl6
Siegel, S.; Acta Crystallographica (1,1948-23,1967) 9 (1956) 827–827; doi:

data_2310669
_publ_section_title
;
 The structures of Cs2 Th Cl6 and Cs2 U Cl6
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              827
_journal_page_last               827
_journal_volume                  9
_journal_year                    1956
_chemical_formula_sum            'Cl6 Cs2 U'
_chemical_name_systematic        'Cs2 U Cl6'
_space_group_IT_number           164
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   7.492
_cell_length_b                   7.492
_cell_length_c                   6.038
_cell_volume                     293.508
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Siegel_ACCRA9_1956_210.cif
_cod_data_source_block           Cl6Cs2U1
_cod_original_cell_volume        293.5076
_cod_original_formula_sum        'Cl6 Cs2 U1'
_cod_database_code               2310669
The Structures of hexagonal Cs Cd Cl3 and tetragonal Cs2 Cd Cl4
Siegel, S.; Gebert, E.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 790–790; doi:

data_2310670
_publ_section_title
;
 The Structures of hexagonal Cs Cd Cl3 and tetragonal Cs2 Cd Cl4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              790
_journal_page_last               790
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Cd Cl3 Cs'
_chemical_name_systematic        'Cs Cd Cl3'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   7.418
_cell_length_b                   7.418
_cell_length_c                   18.39
_cell_volume                     876.367
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Siegel_ACCRA9_1964_154.cif
_cod_data_source_block           Cd1Cl3Cs1
_cod_original_formula_sum        'Cd1 Cl3 Cs1'
_cod_database_code               2310670
The structures of hexagonal Cs Cd Cl3 and tetragonal Cs2 Cd Cl4
Siegel, S.; Gebert, E.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 790–790; doi:

data_2310671
_publ_section_title
;
 The structures of hexagonal Cs Cd Cl3 and tetragonal Cs2 Cd Cl4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              790
_journal_page_last               790
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Cd Cl4 Cs2'
_chemical_name_systematic        'Cs2 Cd Cl4'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.26
_cell_length_b                   5.26
_cell_length_c                   16.88
_cell_volume                     467.029
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Siegel_ACCRA9_1964_155.cif
_cod_data_source_block           Cd1Cl4Cs2
_cod_original_cell_volume        467.0291
_cod_original_formula_sum        'Cd1 Cl4 Cs2'
_cod_database_code               2310671
Influence of lattice interactions on the Jahn-Teller distortion of the [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
Simmons, C.J.; Stratemeier, H.; Riley, M.J.; Hitchman, M.A.; Inorganic Chemistry 45 (2006) 1021–1031; doi:

data_4343906
_publ_section_title
;
 Influence of lattice interactions on the Jahn-Teller distortion of the
 [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2
 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1021
_journal_page_last               1031
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cu H12 K2 O14 Se2'
_chemical_name_systematic        'K2 (Cu (H2 O)6) (Se O4)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 103
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.1617
_cell_length_b                   12.2559
_cell_length_c                   6.3327
_cell_volume                     692.842
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Simmons_INOCAJ_2006_664.cif
_cod_data_source_block           H12Cu1K2O14Se2
_cod_original_cell_volume        692.8419
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H12 Cu1 K2 O14 Se2'
_cod_database_code               4343906
Influence of lattice interactions on the Jahn-Teller distortion of the [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
Simmons, C.J.; Stratemeier, H.; Riley, M.J.; Hitchman, M.A.; Inorganic Chemistry 45 (2006) 1021–1031; doi:

data_4343907
_publ_section_title
;
 Influence of lattice interactions on the Jahn-Teller distortion of the
 [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2
 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1021
_journal_page_last               1031
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cu H12 K2 O14 S2'
_chemical_name_systematic        'K2 (Cu (H2 O)6) (S O4)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.3545
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.0462
_cell_length_b                   12.0492
_cell_length_c                   6.1368
_cell_volume                     648.025
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Simmons_INOCAJ_2006_666.cif
_cod_data_source_block           H12Cu1K2O14S2
_cod_original_cell_volume        648.0248
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H12 Cu1 K2 O14 S2'
_cod_database_code               4343907
Influence of lattice interactions on the Jahn-Teller distortion of the [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
Simmons, C.J.; Stratemeier, H.; Hitchman, M.A.; Riley, M.J.; Inorganic Chemistry 45 (2006) 1021–1031; doi:

data_4343908
_publ_section_title
;
 Influence of lattice interactions on the Jahn-Teller distortion of the
 [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2
 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1021
_journal_page_last               1031
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cu H12 K2 O14 S0.318 Se1.682'
_chemical_name_systematic        'K2 (Cu (H2 O)6) (S O4)0.318 (Se O4)1.682'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 103
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.1345
_cell_length_b                   12.2223
_cell_length_c                   6.3088
_cell_volume                     686.291
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Simmons_INOCAJ_2006_668.cif
_cod_data_source_block           H12Cu1K2O14S0.318Se1.682
_cod_original_cell_volume        686.2911
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H12 Cu1 K2 O14 S0.318 Se1.682'
_cod_database_code               4343908
Influence of lattice interactions on the Jahn-Teller distortion of the [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
Simmons, C.J.; Riley, M.J.; Stratemeier, H.; Hitchman, M.A.; Inorganic Chemistry 45 (2006) 1021–1031; doi:

data_4343909
_publ_section_title
;
 Influence of lattice interactions on the Jahn-Teller distortion of the
 [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2
 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1021
_journal_page_last               1031
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cu H12 K2 O14 S0.356 Se1.644'
_chemical_name_systematic        'K2 (Cu (H2 O)6) (S O4)0.356 (Se O4)1.644'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 103
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.1631
_cell_length_b                   12.2525
_cell_length_c                   6.324
_cell_volume                     691.804
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Simmons_INOCAJ_2006_669.cif
_cod_data_source_block           H12Cu1K2O14S0.356Se1.644
_cod_original_cell_volume        691.8038
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H12 Cu1 K2 O14 S0.356 Se1.644'
_cod_database_code               4343909
Influence of lattice interactions on the Jahn-Teller distortion of the [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
Simmons, C.J.; Stratemeier, H.; Hitchman, M.A.; Riley, M.J.; Inorganic Chemistry 45 (2006) 1021–1031; doi:

data_4343910
_publ_section_title
;
 Influence of lattice interactions on the Jahn-Teller distortion of the
 [Cu (H2 O)6](2+) ion: dependence of the crystal structure of K2 [Cu (H2
 O)6] (S O4)(2x) (Se O4)(2-2x) upon the sulfate/selenate ratio
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1021
_journal_page_last               1031
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'Cu H12 K2 O14 S0.5 Se1.5'
_chemical_name_systematic        'K2 (Cu (H2 O)6) (S O4)0.5 (Se O4)1.5'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 103
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.089
_cell_length_b                   12.1716
_cell_length_c                   6.2848
_cell_volume                     677.453
_citation_journal_id_ASTM        INOCAJ
_cod_data_source_file            Simmons_INOCAJ_2006_670.cif
_cod_data_source_block           H12Cu1K2O14S0.5Se1.5
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H12 Cu1 K2 O14 S0.5 Se1.5'
_cod_database_code               4343910